Chapter 8 Design of Concrete Mixes


 Corey Jasper West
 2 years ago
 Views:
Transcription
1 Chapter 8 Design of Concrete Mixes 1
2 The basic procedure for mix design is applicable to concrete for most purposes including pavements. Concrete mixes should meet; Workability (slump/vebe) Compressive strength Durability (w/c ratio) 2
3 8.1 The workability of concrete Measurement of workability A workable concrete is defined as a concrete suitable for placing and compacting under the site conditions. Slump and Vebe time tests will be used (see Table 3). 3
4 8.1.2 Water content The water content expressed as mass per unit volume of concrete. It is the major factor influencing the workability of concrete. Uncrushed aggregates require a lower water content than crushed aggregates to make concrete of equal workability. The smaller the maximum size of the aggregate the higher the water content needed. 4
5 8.1.2 Water content Table 3 gives typical values of the freewater content for use in the mix design at four different levels of slump or Vebe time, with different types and maximum sizes of aggregate. Figure 6 shows how the fines content of the mix should be reduced as the sand becomes finer, ie as the percentage passing the 600 µm test sieve increases. 5
6 8.1.3 Type and strength class of cement Different types and strength classes of cement have different water requirements to produce pastes of standard consistence. 6
7 8.2 The compressive strength of concrete Age at test and curing conditions The strength is specified at an age of 28 days. The strength development depends on the temperature and humidity conditions during curing. Higher temperatures increase the speed of the chemical reaction and thus the rate of strength development. In order to achieve higher strengths at later ages loss of water from the concrete must be prevented (CURING). Concrete test specimens are stored in water at a constant temperature as specified in standards. 7
8 8.2.2 Type and strength class of cement Class 52.5 Portland cements initially proceeds at a faster rate than in class 42.5 Portland cements; the effect of this on typical concretes having a freewater/cement ratio of 0.5 is shown in Table 2. Information available related to local materials can be used instead of the values given in Table 2. 8
9 8.2.3 Cement strength variation This is due to the variability of cement supplied from different works and to normal variations in production from any one works over a period of time. Standard deviation (s) of the strength of concrete cubes at 28 days made with Portland cement class 42.5 from different works is about 5 N/mm 2. The standard deviation due to the variability of the cement from a single work is about 3 N/mm 2. 9
10 8.2.4 Aggregate type and grading The type and source of the aggregate has a considerable influence on the compressive strength of concrete. Uncrushed coarse aggregate makes a concrete with a lower strength than one with crushed coarse aggregate. Factors such as the type of fine aggregate, the maximum size of aggregate, the overall grading, and particle shape and surface texture, have little direct effect on the compressive strength. Typical strength values when uncrushed or crushed coarse aggregates are used are given in Table 2. 10
11 8.2.5 Relationship between compressive strength and freewater/cement ratio Figure 4 shows the the relationship between the compressive strength and the freewater/ cement ratio. Table 2 gives typical data for a concrete having a free water/ cement ratio of 0.5 to give a datum point on Figure 4 appropriate to the age of test and materials to be used. The strength development shown in Table 2 applies to a concrete with a cement content of about 300 kg/m 3 cured in water at 20 C. Such a mix made with Portland cement class 42.5 has a 7day strength about 70% of that attained at 28 days. Richer mixes initially gain strength more rapidly so that 7day strength may well exceed 75% of the 28day strength. 11
12 8.2.6 Type of mixing Certain types of mixes require a higher degree of workability for efficient operation. Handmixing is likely to produce a lower strength concrete than machinemixed concrete of similar proportions. 12
13 8.3 Variability of concrete strength during production Factors contributing to the overall variation The overall variation in the measured strength of concrete that is obtained during a job can be considered to be made up of three component sources which are:  Variation in the quality of the materials used  Variation in the mix proportions due to the batching process  Variation due to sampling and testing 13
14 8.4 The distribution of results Variation in concrete strengths follows the normal distribution such as that shown in Figure l. The proportion of results less than some specified value is represented by the area beneath the curve to the lefthand side of a vertical line drawn through the specified value. This normal distribution curve is symmetrical about its mean, has a precise mathematical equation and is completely specified by two parameters, its mean m and its standard deviation s. The standard deviation is a measure of the variability calculated from the equation: where x = an individual result n = the number of results m= the mean of the n results 14
15 Example F c1 =45 MPa F c2 =48 MPa F c3 =44 MPa What is standard (s) deviation and average of these samples? s = F cav = Average of results 15
16 8.4 The distribution of results Standard deviation increases as the specified characteristic strength increases up to a particular level. This type of relationship is shown in Figure 3, the standard deviation being independent of the specified characteristic strength above 20 N/mm 2. 16
17 8.5 Characteristic strength Concrete cube strengths follow the normal distribution. There is therefore always the probability that a result will be obtained less than the specified strength. Specify the quality of concrete not as a minimum strength but as a characteristic strength below which a specified proportion of the test results, often called defectives, may be expected to fall. 17
18 8.6 Margin and target mean strength where f m = the target mean strength f c = the specified characteristic strength ks = the margin, which is the product of: f m = f c + k s s = the standard deviation, k = a constant The constant k is derived from the mathematics of the normal distribution and increases as the proportion of defectives is decreased, thus: k for 10% defectives = 1.28 k for 5% defectives = 1.64 k for 2.5% defectives = 1.96 k for 1% defectives =
19 8.7 The Mix Design Process Flow chart of procedures A suitable mix design form for recording the values derived is shown in Table 1. Initial information is divided into two categories:  specified variables, the values of which are usually nominated in specifications,  additional information, which is normally available to the producer of the concrete. This initial information is also subdivided into two categories:  the mix parameters  the final unit proportions 19
20 8.7 The Mix Design Process Flow chart of procedures Stage 1 deals with strength leading to the freewater/cement ratio Stage 2 deals with workability leading to the freewater Content Stage 3 combines the results of Stages 1 and 2 to give the cement content Stage 4 deals with the determination of the total aggregate content Stage 5 deals with the selection of the fine and coarse aggregate contents The mix design form shown in Table 1 is subdivided into the same five stages and the separate item numbers. 20
21 8.7.2 Selection of target water/cement ratio (Stage 1) If previous information concerning the variability of strength tests comprises fewer than 20 results, the standard deviation to be adopted should be that obtained from line A in Figure 3. If previous information is available consisting of 20 or more results, the standard deviation of such results may be used provided that this value is not less than the appropriate value obtained from line B. The margin can then be derived from calculation C1: M = k x s... C1 Where: M = the margin k = a value appropriate to the percentage defectives permitted below the characteristic strength s = the standard deviation. (The margin itself may be specified directly). 21
22 8.7.2 Selection of target water/cement ratio (Stage 1) Calculation C2 determines the target mean strength: f m = f c + M...C2 Where: f m = the target mean strength f c = the specified characteristic strength M = the margin 22
23 8.7.2 Selection of target water/cement ratio (Stage 1) A value is obtained from Table 2 for the strength of a mix made with a freewater/cement ratio of 0.5 according to the specified age, the strength class of the cement and the aggregate to be used. This strength value is then plotted on Figure 4 and the freewater/cement ratio can then be read from the abscissa. Compare this value with maximum freewater/cement ratio that may be specified and the lower of these two values used. 23
24 8.7.3 Selection of freewater content (Stage 2) Consists of determining the freewater content from Table 3 depending upon the type and maximum size of the aggregate to give a concrete of the specified slump or Vebe time Determination of cement content (Stage 3) Cement content = freewater content / freewater/cement ratio C3 The result should be checked against any maximum or minimum value that may be specified. 24
25 8.7.5 Determination of total aggregate content (Stage 4) Estimate of the density of the fully compacted concrete which is obtained from Figure 5. If no information is available assume a value of 2.6 for uncrushed aggregate and 2.7 for crushed aggregate. Total aggregate content is determined from calculation C4: Total aggregate content = D C W where D = the wet density of concrete (kg/m 3 ) C = the cement content (kg/m 3 ) W = the freewater content (kg/m 3 ) C4 25
26 8.7.6 Selection of fine and coarse aggregate contents (Stage 5) Involves deciding how much of the total aggregate should consist of materials smaller than 5 mm. Figure 6 shows recommended values for the proportion of fine aggregate depending on the maximum size of aggregate, the workability level, the grading of the fine aggregate (defined by its percentage passing a 600 µm sieve) and the freewater/cement ratio. The final calculation, C5, to determine the fine and coarse aggregate contents: Fine aggregate content = (total aggregate content) x (proportion of fines) C5 Coarse aggregate content = (total aggregate content) (fine aggregate content)..c5 26
27 8.7.6 Selection of fine and coarse aggregate contents (Stage 5) The coarse aggregate content itself can be subdivided if single sized 10, 20 and 40 mm materials are to be combined. 1 : 2 for combination of 10 and 20 mm 1 : 1.5 : 3 for combination of 10, 20 and 40 mm 27
28 8.8 Trial mixes use the trial mix proportions in the production mixes modify the trial mix proportions slightly in the production mixes prepare further trial mixes incorporating major changes to the mix proportions 28
29 8.8.1 Production of trial mixes Typically, a 50 litre (0.05 m3) mix is sufficient to make six cubes of 150 mm side and to carry out, separately, measurements of slump, Vebe time and density. The individual batch quantities (in kg) would then be equal to the appropriate contents, multiplied by The British Standard allows the use of aggregates in any one of four moisture conditions, ie (a) ovendry, (b) airdried, (c) saturated surfacedry, or (d) saturated by soaking in water for at least 24 hours. 29
30 8.8.2 Tests on trial mixes Slump Vebe time Density Make test cubes Apply Normal curing on test cubes Compression testing of cubes 30
31 8.8.3 Adjustments to mix proportions (workability) Workability During the mixing of the trial mix an experienced technician is able to adjust the water content by inspection if the workability of the mix is much outside the specified range. It is thus useful, initially, to withhold a small proportion, say 10%, of the mix water until the technician has assessed visually that its addition is needed to achieve the required workability. Furthermore, if at the designed water content the workability of the trial mix appears below that required, additional water should be added to obtain the required workability. 31
32 After completion of the mixing cycle and workability measurements a change of water content may still be needed, either for use in the production mix or for a further trial mix, and this can be estimated by reference to Table 3. During the measurement of workability the concrete should also be assessed subjectively for its other rheological properties; this may indicate a need to change the relative aggregate proportions 32
33 8.8.3 Adjustments to mix proportions (density) Density After the density of the fresh concrete is measured, the resultant value is compared with the density value used during the design. If there is an appreciable difference, the constituent contents will differ from those intended in the initial design. In this case, the initial design values should be corrected by the ratio of measured density to assumed density in order to determine the actual masses. 33
34 8.8.3 Adjustments to mix proportions (strength) When results of the strength tests become available they are compared with the target mean strength. If necessary an adjustment is made to the water/cement ratio by using the curves of Figure 4. Two examples of this adjustment are shown in Figure 7, where: A represents the reference data given in Table 2 B represents the freewater/cement ratio estimated for the trial mix B' represents the actual freewater/cement ratio used in the trial mix when different from B. C represents the strength result of the test specimens made from the trial mix. D represents the new estimate of the freewater/cement ratio required to give the target mean strength. Minor adjustments may be made to the mix proportions for use in production mixes without the need to carry out further trials. Exceptionally, when large adjustments seem to be necessary to the water/cement ratio it is advisable to make a second trial mix using the revised proportions and recalculated batch quantities based on the updated value for density of the mix. 34
35 8.9 Examples of mix design Example 1: unrestricted design Characteristic compressive strength (f c ) = 30 N/mm 2 at 28 days, with a 2.5% defective rate (k = 1.96) Portland cement class 42.5 Slump required = mm Maximum aggregate size = 20 mm (uncrushed) Fine aggregate: 70% passing 600 µm sieve (uncrushed) Maximum freew/c ratio = 0.55 Minimum cement content = 290 kg/m 3 Maximum cement content = not specified. 35
36 Example 2: mix restricted by maximum water/cement ratio CALCULATE MIX PROPORTIONS FOR FOLLOWING CONDITIONS: Characteristic compressive strength (f c ), 25 N/mm 2 at 28 days Portland cement class 42.5 Slump required, mm Maximum aggregate size, 40 mm (fine and coarse uncrushed) Maximum freewater/cement ratio, 0.50 Minimum cement content, 290 kg/m3 There are no previous control data but a margin of 10 N/mm2 is specified and is used in Item 1.3. The following information is known concerning the aggregates to be used and the data are entered under the relevant items on the mix design form, as shown in Table 5: Aggregate relative density = 2.5 Item 4.1 Fine aggregate, 90% passing a 600µm sieve 36
37 Example 4: Restricted by maximum cement content CALCULATE MIX PROPORTIONS FOR CONDITIONS GIVEN BELOW: Characteristic compressive strength (f c ), 50 N/mm2 at 7 days, defective rate 1% (k = 2.33) Portland cement class 52.5 Item 1.5 Slump required, mm Item 2.1 Maximum aggregate size, 10 mm Item 2.2 Maximum cement content, 550 kg/m3 Item 3.2 Previous control data indicated an expected standard deviation of 5 N/mm2 and this is used in Item
38 k for 10% defectives = 1.28 k for 5% defectives = 1.64 k for 2.5% defectives = 1.96 k for 1% defectives =
39 39
40 Figure 3. Relationship between standard deviation and characteristic strength 40
41 Figure 4. Relation between compressive strength and freewater/cement ratio 41
42 Table 2 42
43 Table 3 43
44 Figure 5. Estimated wet density of fully compacted concrete. 44
45 Figure 6. Recommended proportions of fine aggregate according to percentage passing 600 m sieve (Dmax 10 mm). 45
46 Figure 6. Recommended proportions of fine aggregate according to percentage passing 600 m sieve (D max 20 mm). 46
47 Figure 6. Recommended proportions of fine aggregate according to percentage passing 600 m sieve (D max 40 mm). 47
48 Table 4 48
49 Table 5 49
50 Table 6 50
51 Table 7 51
52 Mix Design Problems 1. Calculate the quantities of cement, water, fine aggregate and coarse aggregate per trial mix of 0.05 m3 for the following specifications. Characteristic compressive strength = 30 MPa at 28 days; Defective rate = 5%; Cement = Cement strength class 42.5; Slump required = mm; Max. Aggregate size = 20 mm; Coarse aggregate UNCRUSHED (10, 20 mm), fine aggregate UNCRUSHED (70% pass 600 microns)); Maximum allowable free water/cement ratio = 0.55; Minimum allowable cement content = 290 kg/m3 52
53 Mix Design Problems 2. Calculate the quantities of cement, water, fine aggregate and coarse aggregate per trial mix of 0.08 m3 for the following specifications. Characteristic compressive strength = 15 MPa at 28 days; Defective rate = 5%; Cement = Cement strength class 42.5; Slump required = mm; Max. Aggregate size = 40 mm; Coarse aggregate UNCRUSHED (10, mm), fine aggregate UNCRUSHED (90% pass 600 microns); Relative density of aggregates = 2.50; Maximum allowable free water/cement ratio = 0.50; Minimum allowable cement content = 290 kg/m3 53
54 Mix Design Problems 3. Calculate the quantities of cement, water, fine aggregate and coarse aggregate per trial mix of 0.08 m3 for the following specifications. Characteristic compressive strength = 50 MPa at 28 days; Defective rate = 1%; Cement strength class 42.5; Slump required = mm; Max. Aggregate size = 10 mm; Coarse aggregate CRUSHED (10 mm), fine aggregate CRUSHED (85% pass 600 microns) Maximum allowable free water/cement ratio = 0.50; Maximum allowable cement content = 550 kg/m3 54
55 Problem with different moisture conditions: 4. Calculate the quantities of cement, water, fine aggregate, and coarse aggregate per trial mix of 0.05 m3 for the following specifications. Characteristic compressive strength = 30 MPa at 28 days; Defective rate = 5%; Cement strength class 42.5; Slump required = 100 mm; Max. Aggregate size = 40 mm; Coarse aggregate UNCRUSHED (10, 20, 40mm), fine aggregate UNCRUSHED (80% pass 600 microns); Maximum allowable free water/cement ratio = 0.50; Minimum allowable cement content = 290 kg/m3 55
56 Problem with different moisture conditions: 5. Calculate the quantities of cement, water, fine aggregate, and coarse aggregate per trial mix of 1 m3 for the following specifications. Target mean compressive strength = 30 MPa at 7 days; Cement strength class 42.5; Slump required = 100 mm; Max. Aggregate size = 20 mm; Specific gravity of aggregates = 2.65; Coarse aggregate UNCRUSHED (10, 20mm), fine aggregate CRUSHED (50% pass 600 micros); Maximum allowable free water/cement ratio = 0.40; Minimum allowable cement content = 275 kg/m3; Absorption of fine aggregate = 1.0%; Absorption of coarse aggregate = 1.0%; Total Moisture content of coarse aggregate = 3.0%; Total Moisture content of fine aggregate = 3.0% 56
57 Problem with different moisture conditions: 6. The following requirements are specified for the mix design as follows; Make a trial mix of 0.05 m3 concrete. Show your results on Table 1. Characteristic compressive strength = 20 MPa at 28 days; Defective rate = 10%; Cement strength class 42.5; Slump required = 65 mm; Max. Aggregate size = 40 mm; Coarse aggregate CRUSHED (all in aggregate), fine aggregate UNCRUSHED (70% pass 600 microns) Relative density of aggregates = 2.65; Maximum allowable free water/cement ratio = 0.55; Minimum allowable cement content = 250 kg/m3 ; Maximum allowable cement content = 350 kg/m3 ; Absorption of fine aggregate = 2%; Absorption of coarse aggregate = 1.1% Total Moisture content of coarse aggregate = 2.2%; Total Moisture content of fine aggregate = 1.5% 57
58 Problem with different moisture conditions: 7. The following requirements are specified for the mix design as follows; Characteristic compressive strength = 35 MPa at 28 days; Defective rate = 2.5%; Cement strength class 52.5; Slump required = 100 mm; Max. Aggregate size = 20 mm; Coarse aggregate CRUSHED (10, 20mm), fine aggregate UNCRUSHED (55% pass 600 microns) Relative density of aggregates = 2.75; Maximum allowable free water/cement ratio = 0.50; Minimum allowable cement content = 285 kg/m3 ; Maximum allowable cement content = 400 kg/m3; Absorption of fine aggregate = 1.8%; Absorption of coarse aggregate = 1.2% Total Moisture content of coarse aggregate = 2.3%; Total Moisture content of fine aggregate = 3.4% Make a trial mix of 0.08 m3 concrete. Show your results on Table 1. 58
59 Problem with different moisture conditions: 8. The following requirements are specified for the mix design as follows; Characteristic compressive strength = 25 MPa at 28 days; Defective rate = 5%; Cement strength class 42.5; Slump required = 35 mm; Max. Aggregate size = 20 mm; Coarse aggregate CRUSHED (all in aggregate), fine aggregate CRUSHED (90% pass 600 microns) Relative density of aggregates = 2.75; Maximum allowable free water/cement ratio = 0.55; Minimum allowable cement content = 250 kg/m3; Absorption of fine aggregate = 1.5%; Absorption of coarse aggregate = 1.0%; Total Moisture content of coarse aggregate = 3.0% Total Moisture content of fine aggregate = 2.0% Make a trial mix of 0.05 m3 concrete. Show your results on Table 1. 59
60 Problem with different moisture conditions: 9. The following requirements are specified for the mix design as follows; Target, mean compressive strength = 40 MPa at 28 days; Cement strength class 52.5; VeBe required = 12 sec; Max. Aggregate size = 25 mm; Coarse aggregate CRUSHED (all in aggregate), fine aggregate CRUSHED (55% pass 600 microns); Relative density of aggregates = 2.65; Maximum allowable free water/cement ratio = 0.55; Minimum allowable cement content = 350 kg/m3; Maximum allowable cement content = 500 kg/m3; Absorption of coarse aggregate = 2.0%; Total Moisture content of coarse aggregate = 1.5% Surface Moisture content of fine aggregate = 2.5% Make a trial mix of 0.05 m3 concrete. Show your results on Table 1. 60
APPENDIX 2 MIX DESIGNS. Chapter 4: mix design calculation sheet for 40 N/mm 2 strength)
APPENDIX 2 MIX DESIG All mixes in this study were designed in accordance with the Building Research Establishment (BRE 1992) method, recommended by the UK Department of the Environment. Reference should
More informationNOTE: FOR PROJECTS REQUIRING CONTRACTOR MIX DESIGN, THE DESIGN PROCEDURES ARE SPECIFIED IN THE SPECIAL PROVISIONS OF THE CONTRACT.
September 1, 2003 CONCRETE MANUAL 5694.300 MIX DESIGN 5694.300 NOTE: FOR PROJECTS REQUIRING CONTRACTOR MIX DESIGN, THE DESIGN PROCEDURES ARE SPECIFIED IN THE SPECIAL PROVISIONS OF THE CONTRACT. 5694.301
More informationHow To Make Concrete At Site? M 25 Example
How To Make Concrete At Site? M 25 Example By Er. Kaushal Kishore, Materials Engineer, Roorkee PORTLAND CEMENT: Joseph Aspdin, a mason at Leeds prepared a cement in 1824 by heating a mixture of finelydivided
More informationConcrete Mix Design Guide
The following is a design guide for selecting proportions for initial concrete mix design for normal weight concrete. This guide references ACI 211.191 (Reapproved 2009), Standard Practice for Selecting
More informationImportance of quality assurance of materials for construction work
Importance of quality assurance of materials for construction work R.Savitha Building Materials Research and Testing Division, National Building Research Organization ABSTRACT: Quality assurance of building
More informationStrength and Workability Characteristics of Concrete by Using Different Super Plasticizers
International Journal of Materials Engineering 12, 2(1): 711 DOI: 1.923/j.ijme.11.2 Strength and Workability Characteristics of Concrete by Using Different Super Plasticizers Venu Malagavelli *, Neelakanteswara
More informationEXPERIMENTAL INVESTIGATION ON BEHAVIOUR OF NANO CONCRETE
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 315 320, Article ID: IJCIET_07_02_027 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationPerformance of Recycled Asphalt Pavement as Coarse Aggregate in Concrete
Leonardo Electronic Journal of Practices and Technologies ISSN 15831078 Issue 17, JulyDecember 2010 p. 4758 Performance of Recycled Asphalt Pavement as Coarse Aggregate in Concrete Department of Civil
More informationCONCRETE TECHNOLOGY LABORATORY
CONCRETE TECHNOLOGY LABORATORY DEPARTMENT OF CIVIL ENGINEERING CHULALONGKORN UNIVERSITY Tested by... ID. No.... Date... Graded by... TEST No. C2 PROPERTIES OF AGGREGATE Part A Specific Gravity and Absorption
More informationCHAPTER 3 FLY ASH BASED GEOPOLYMER CONCRETE
29 CHAPTER 3 FLY ASH BASED GEOPOLYMER CONCRETE 3.1 GENERAL The fresh and hardened properties such as workability, density, compressive strength, split tensile strength and flexural strength of fly ash
More information"EFFECTS OF WATER TO CEMENTITIOUS RATIO ON COMPRESSIVE STRENGTH OF CEMENT MORTAR CONTAINING FLY ASH"*
"EFFECTS OF WATER TO CEMENTITIOUS RATIO ON COMPRESSIVE STRENGTH OF CEMENT MORTAR CONTAINING FLY ASH"* By Tarun R. Naik, Ph.D., P.E. Director, Center for ByProducts Utilization Shiw S. Singh, Ph.D., P.E.
More informationOptimization of Mix Proportion of High Performance Mortar for Structural Applications
American J. of Engineering and Applied Sciences 3 (4): 643649, 2010 ISSN 19417020 2010 Science Publications Optimization of Mix Proportion of High Performance Mortar for Structural Applications Cheah
More informationPROPERTIES AND MIX DESIGNATIONS 5694.200
September 1, 2003 CONCRETE MANUAL 5694.200 5694.210 PROPERTIES OF CONCRETE PROPERTIES AND MIX DESIGNATIONS 5694.200 Inspectors should familiarize themselves with the most important properties of concrete:
More information1.5 Concrete (Part I)
1.5 Concrete (Part I) This section covers the following topics. Constituents of Concrete Properties of Hardened Concrete (Part I) 1.5.1 Constituents of Concrete Introduction Concrete is a composite material
More informationAPPRAISAL ON THE STRENGTH OF CONCRETE PRODUCED WITH VARYING AGGREGATE SIZE
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 3, May June 2016, pp. 233 240, Article ID: IJCIET_07_03_023 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=3
More informationEXPERIMENT NO.1. : Vicat s apparatus, plunger
EXPERIMENT NO.1 Name of experiment:to determine the percentage of water for normal consistency for a given sample of cement Apparatus : Vicat s apparatus with plunger of 10mm dia, measuring cylinder, weighing
More informationSTRENGTH OF CONCRETE INCORPORATING AGGREGATES RECYCLED FROM DEMOLITION WASTE
STRENGTH OF CONCRETE INCORPORATING AGGREGATES RECYCLED FROM DEMOLITION WASTE R. Kumutha and K. Vijai Department of Civil Engineering, Sethu Institute of Technology, Pulloor, Kariapatti, India EMail: kumuthar@yahoo.co.in,
More informationAGGREGATES FOR CONCRETE
ACI Education Bulletin E199 AGGREGATES FOR CONCRETE Developed by Committee E701, s for Concrete Construction Charles K. Nmai, Chairman David M. Suchorski, Secretary Patrick L. McDowell Chairman, document
More informationREFERENCE TO STANDARD SPECIFICATIONS CONCRETE AGGREGATE TESTS ON CONCRETE AGGREGATE CEMENT 4
06005_Jan06_2014.pdf Page 1 of 14 INDEX Page 060051 REFERENCE TO STANDARD SPECIFICATIONS 2 060052 CONCRETE AGGREGATE 2 060053 TESTS ON CONCRETE AGGREGATE 3 060054 CEMENT 4 060055 PROVIDING CHEMICAL
More informationShotcrete Quality Control and Testing for an Underground Mine in Canada
Shotcrete Quality Control and Testing for an Underground Mine in Canada By Dudley R. (Rusty) Morgan and Mazin Ezzet AMEC Earth & Environmental, a division of AMEC Americas Limited SHOTCRETE FOR AFRICA
More informationExperimental Study on Properties of Nofine Concrete
Research Paper Volume 2 Issue 10 June 2015 International Journal of Informative & Futuristic Research ISSN (Online): 23471697 Experimental Study on Properties of Nofine Paper ID IJIFR/ V2/ E10/ 055 Page
More informationFREE MOISTURE AND WATER ABSORPTION IN AGGREGATE FOR CONCRETE
Test Procedure for FREE MOISTURE AND WATER ABSORPTION IN AGGREGATE FOR TxDOT Designation: Tex409A Effective Date: August 1999 1. SCOPE 1.1 This test is a rapid procedure for field determining the percentage
More informationPolymerModified Mortars And Concrete Mix Design
PolymerModified Mortars And Concrete Mix Design By Kaushal Kishore Materials Engineer, Roorkee Polymermodified Concrete (PMC) has also been called polymerportland cementconcrete (PPCC) and latexmodified
More informationEvaluation of M35 and M40 grades of concrete by ACI, DOE, USBR and BIS methods of mix design
Evaluation of M35 and M40 grades of concrete by ACI, DOE, USBR and BIS methods of mix design Sharandeep Singh 1, Dr.Hemant Sood 2 1 M. E. Scholar, CIVIL Engineering, NITTTR, Chandigarh, India 2Professor
More informationEFFECT OF NANOSILICA ON CONCRETE CONTAINING METAKAOLIN
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 1, JanFeb 2016, pp. 104112, Article ID: IJCIET_07_01_009 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=1
More informationEffect of Fine Aggregate Particles on Compressive Strength of Cement Mortar
Page8 Effect of Fine Aggregate Particles on Compressive Strength of Cement Mortar ABSTRACT: Chandra Prakash Bastani* & R. Kansal** *M..E.IV Sem.(CTM) Student **Professor & Head, Department Of Civil Engineering,
More informationEffect of basalt aggregates and plasticizer on the compressive strength of concrete
International Journal of Engineering & Technology, 4 (4) (2015) 520525 www.sciencepubco.com/index.php/ijet Science Publishing Corporation doi: 10.14419/ijet.v4i4.4932 Research Paper Effect of basalt aggregates
More informationA COMPREHENSIVE STUDY ON PARTIAL REPLACEMENT OF CEMENT WITH SUGARCANE BAGASSE ASH, RICE HUSK ASH & STONE DUST
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 3, May June 2016, pp. 163 172, Article ID: IJCIET_07_03_016 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=3
More informationEffect of Specific Gravity on Aggregate Varies the Weight Of Concrete Cube
Effect of Specific Gravity on Aggregate Varies the Weight Of Concrete Balamurali Arumugam, Senior Lecturer (Civil), ISTE124, Department of Civil Engineering, LathaMathavan Polytechnic College, Alagarkovil,
More informationLab 1 Concrete Proportioning, Mixing, and Testing
Lab 1 Concrete Proportioning, Mixing, and Testing Supplemental Lab manual Objectives Concepts Background Experimental Procedure Report Requirements Discussion Prepared By Mutlu Ozer Objectives Students
More informationUse of building rubbles as recycled aggregates
Cement and Concrete Research 33 (2003) 125 132 Use of building rubbles as recycled s HowJi Chen*, Tsong Yen, KuanHung Chen Department of Civil Engineering, National ChungHsing University, 250, KuoKuang
More information1.1 SCOPE: 1.2 DEFINITIONS:
PART 1 GENERAL 1.1 SCOPE: A. This work consists of establishing the JMF for HMAC for use in road and street constructions and/or repairs. Once established and accepted the JMF will be used to determine
More informationSTATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENT 1015 COMPACTION TESTING OF UNBOUND MATERIALS. July 18, 2014
STATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENT 1015 COMPACTION TESTING OF UNBOUND MATERIALS July 18, 2014 1015.01 General 1015.02 Definitions 1015.03 Referenced Standards 1015.04 Equipment 1015.05
More informationMETHOD OF TEST FOR MOISTUREDENSITY RELATIONSHIP OF SOILS USING 2.5 kg RAMMER AND 305 mm DROP
Laboratory Testing Manual Date: 96 05 01 Page 1 of 7 METHOD OF TEST FOR MOISTUREDENSITY RELATIONSHIP OF SOILS USING 2.5 kg RAMMER AND 305 mm DROP 1. SCOPE 1.1 This method covers the determination of the
More informationGRADATION OF AGGREGATE FOR CONCRETE BLOCK
GRADATION OF AGGREGATE FOR CONCRETE BLOCK Although numerous papers have been written concerning the proper gradation for concrete mixes, they have generally dealt with plastic mixes, and very little published
More informationSATURATED SURFACEDRY SPECIFIC GRAVITY AND ABSORPTION OF AGGREGATES
Test Procedure for SATURATED SURFACEDRY SPECIFIC GRAVITY AND ABSORPTION OF TxDOT Designation: Tex403A Effective Date: August 1999 1. SCOPE 1.1 This method determines the saturated surfacedry (SSD)
More informationInfluence of fly ash and its mean particle size on certain engineering properties of cement composite mortars
Cement and Concrete Research 35 (2005) 1128 1134 Influence of fly ash and its mean particle size on certain engineering properties of cement composite mortars Gengying Li a, *, Xiaozhong Wu b a Department
More informationEXPERIMENTAL STUDY OF EFFECT OF SODIUM SILICATE (NA 2 SIO 3 ) ON PROPERTIES OF CONCRETE
International Journal of Civil Engineering and Technology (IJCIET Volume 6, Issue 12, Dec 2015, pp. 3947, Article ID: IJCIET_06_12_004 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=12
More informationDurability of block work: the effect of varying water/cement ratio of mortar joint
Available online at www.pelagiaresearchlibrary.com Advances in Applied Science Research, 2012, ():1848185 Durability of block work: the effect of varying water/cement ratio of mortar joint Nwofor, T.C.
More informationComparison of strength and other factors of concrete by replacing normal aggregates with demolished material and plastic aggregate
3rd International Conference on Electrical, Electronics, Engineering Trends, Communication, Optimization and Sciences Comparison of strength and other factors of concrete by replacing normal aggregates
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationCEL 774 IIT DELHI Construction practices. ( Lecture 13) Concrete: Production B. Bhattacharjee CIVIL ENGINEERING DEPARTMENT IIT DELHI
CEL 774 IIT DELHI Construction practices ( Lecture 13) Concrete: Production CIVIL ENGINEERING DEPARTMENT IIT DELHI 1 General Outline Concrete Production. Production Process Batching. Mixing. 2 What is
More informationSPECIFIC GRAVITY OF COARSE AGGREGATE AASHTO T 85
SPECIFIC GRAVITY OF COARSE AGGREGATE AASHTO T 85 GLOSSARY Absorption: The increase in weight due to water contained in the pores of the material. Bulk Specific Gravity (also known as Bulk Dry Specific
More informationAPPLICATION BASED MIX PROPORTIONING FOR SELFCOMPACTING CONCRETE
APPLICATION BASED MIX PROPORTIONING FOR SELFCOMPACTING CONCRETE Anirwan Sengupta*, IIT Madras, Chennai, India Manu Santhanam, IIT Madras, Chennai, India 31st Conference on OUR WORLD IN CONCRETE & STRUCTURES:
More informationQuality control: AnnexA.
Quality control: Quality of the constructed work has been checked by our staff as per frequency and provision mentioned section 900 in MoRT&H and as per provision mentioned in Concession Agreement. The
More informationCHAPTER 4 CONCRETE TRAINING AND QUALIFICATIONPROGRAM
Concrete Training Qualification Program Topic No. 700000001 Effective: July 1, 2002 Construction Training and Qualification Manual Revision: March 22, 2011 Concrete Training and Qualification Program
More informationSieve Analysis of Aggregates
Revised 2007, WKS Datasheet No. 30 MOHAWK COLLEGE OF APPLIED ARTS AND TECHNOLOGY BUILDING AND CONSTRUCTION SCIENCES DEPARTMENT Sieve Analysis of Aggregates INTRODUCTION The evaluation of the distribution
More informationReUse of Polyethylene Plastic Waste In Concrete
ReUse of Polyethylene Plastic Waste In Concrete 1 M Mahesh, 2 B Venkat Narsimha Rao, 3 CH. Satya Sri 1 Assistant Professors, 2 Assistant Professors, 3 Assistant Professors Department of Civil Engineering,
More informationFLEXURAL AND TENSILE STRENGTH PROPERTIES OF CONCRETE USING LATERITIC SAND AND QUARRY DUST AS FINE AGGREGATE
FLEXURAL AND TENSILE STRENGTH PROPERTIES OF CONCRETE USING LATERITIC SAND AND QUARRY DUST AS FINE AGGREGATE Joseph. O. Ukpata 1 and Maurice. E. Ephraim 2 1 Department of Civil Engineering, Cross River
More informationACCELERATING ADMIXTURE RAPIDITE ITS EFFECT ON PROPERTIES OF CONCRETE
International Journal of Civil Engineering and Technology (IJCIET Volume 6, Issue 12, Dec 215, pp. 5865, Article ID: IJCIET_6_12_6 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=12
More informationCity of Regina Standard Construction Specification SECTION 2325 SUPPLY OF ASPHALTIC CONCRETE 1.0 GENERAL. 1.1 Scope
1.0 GENERAL 1.1 Scope 2.0 PRODUCTS 1.1.1 The asphaltic concrete shall consist of a homogeneous mixture of mineral aggregate, filler and asphaltic binder, combined in accordance with these Specifications.
More informationAnalysis of M35 and M40 grades of concrete by ACI and USBR methods of mix design on replacing fine aggregates with stone dust
Analysis of M35 and M40 s of concrete by and methods of mix design on replacing fine aggregates with stone dust Satwinder Singh 1, Dr. Hemant Sood 2 1 M. E. Scholar, Civil Engineering, NITTTR, Chandigarh,
More informationAcceptance testing and criteria for ready mixed concrete in Hong Kong
Acceptance testing and criteria for ready mixed concrete in Hong Kong Albert K.H. Kwan and Isaac S.K. Ling Department of Civil Engineering The University of Hong Kong 1 Outline Introduction Producer s
More informationAsphalt concrete mix design
CEEN 3144 Construction Materials Asphalt concrete mix design Francisco Aguíñiga Assistant Professor Civil Engineering Program Texas A&M University Kingsville Page 1 Asphalt concrete Hotmix asphalt Asphalt
More informationCONCRETE AND JOINTS IN CONCRETE
GENERAL SPECIFICATION FOR CIVIL ENGINEERING WORKS SECTION 16 CONCRETE AND JOINTS IN CONCRETE 16.1 16.2 2006 Edition SECTION 16 CONCRETE AND JOINTS IN CONCRETE PART 1: CONCRETE WORKS GENERAL Sprayed concrete
More informationStudy on durability of high performance concrete with industrial wastes
Peerreviewed & Open access journal ISSN: 18041191 www.pieb.cz ATI  Applied Technologies & Innovations Volume 2 Issue 2 August 2010 pp. 1928 Study on durability of high performance concrete with industrial
More informationDENSITY (UNIT WEIGHT), YIELD, AND AIR CONTENT (GRAVIMETRIC) OF CONCRETE FOP FOR AASHTO T 121 (11)
DENSITY (UNIT WEIGHT), YIELD, AND AIR CONTENT (GRAVIMETRIC) OF CONCRETE FOP FOR AASHTO T 121 (11) Scope This procedure covers the determination of density, or unit weight, of freshly mixed concrete in
More informationASPHALT CONCRETE PAVING
CITY OF BRAMPTON LANDSCAPE SPECIFICATIONS SECTION 027431 PART 1 GENERAL 1.1 Related Work.1 All Division 1 Specification Sections.2 Section 01330 Submittals.3 Section 01450 Quality Control & Inspection.4
More informationCrack the Code on your Concrete Delivery Ticket CONEXPO CON/AGG 3/6/2014
Crack the Code On Your Delivery Ticket Description: Every load of concrete comes with a delivery ticket that is full of useful information, if you know how to crack the secret code! Critical information
More informationSTRENGTH PROPERTIES OF GLASS FIBRE CONCRETE
STRENGTH PROPERTIES OF GLASS FIBRE CONCRETE Chandramouli K. 1, Srinivasa Rao P. 2, Pannirselvam N. 3, Seshadri Sekhar T. 4 and Sravana P. 2 1 Priyadrashini Institute of Technology for Women, Tenali, Guntur,
More informationConcrete Technology Department of Civil Engineering Prof. B. Bhattacharjee Indian Institute of Technology, Delhi
Concrete Technology Department of Civil Engineering Prof. B. Bhattacharjee Indian Institute of Technology, Delhi Lecture 19 Batching and Mixing of Concrete: General Principles So, after looking choose
More informationMechanical Properties and Freezethaw Resistance of FiberMixed Spraying Mortar
Mechanical Properties and Freezethaw Resistance of FiberMixed Spraying Mortar S. YOSHIDA, Civil Engineering Research Institute of Hokkaido, Japan F. TAGUCHI, Civil Engineering Research Institute of Hokkaido,
More informationGuideline for Application and Use of High Performance Concrete. in Projects of Ministry of Transportation Kingdom of Saudi Arabia
Guideline for Application and Use of High Performance Concrete in Projects of Ministry of Transportation Kingdom of Saudi Arabia Rajab 1431 H July 2010 Preface By H.E.Dr.Jobarah bin Eid AlSuraisry
More informationStone crusher dust as a fine aggregate in Concrete for paving blocks
Stone crusher dust as a fine aggregate in Concrete for paving blocks Radhikesh P. Nanda 1, Amiya K. Das 2, Moharana.N.C 3 1 Associate Professor, Department of Civil Engineering, NIT Durgapur, Durgapur
More informationNorthEast Transportation Training and Certification Program (NETTCP) Course Registration Form
(NETTCP) Course Registration Form Interim Certification (Cost $300 members / $425 nonmembers) HMA Plant Technician* HMA Paving Inspector* Soils & Aggregate Inspector* Soils & Aggregate Lab Technician*
More informationINFLUENCE OF STEEL FIBERS AS ADMIX IN NORMAL CONCRETE MIX
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 1, JanFeb 2016, pp. 93103, Article ID: IJCIET_07_01_008 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=1
More informationDEPARTMENT of INFRASTRUCTURE, ENERGY and RESOURCES, TASMANIA GENERAL SPECIFICATION. G4  COMPACTION ASSESSMENT March 1995
DEPARTMENT of INFRASTRUCTURE, ENERGY and RESOURCES, TASMANIA GENERAL SPECIFICATION G4  COMPACTION ASSESSMENT March 1995 INDEX Page G4.1 SCOPE 2 G4.2 DEFINITIONS 2 G4.3 TEST METHODS 3 G4.4 FIELD TESTING
More informationStandard Specification for Concrete Made by Volumetric Batching and Continuous Mixing 1
Designation: 685/ 685M 01 Standard Specification for oncrete Made by Volumetric Batching and ontinuous Mixing 1 This standard is issued under the fixed designation 685/ 685M; the number immediately following
More informationEffect of Curing Temperature on Mortar Based on Sustainable Concrete Material s and PolyCarboxylate Superplasticizer
Jan. 2014, Volume 8, No. 1 (Serial No. 74), pp. 6672 Journal of Civil Engineering and Architecture, ISSN 19347359, USA D DAVID PUBLISHING Effect of Curing Temperature on Mortar Based on Sustainable Concrete
More informationCity of Regina Standard Construction Specification SECTION 2500 SUPPLY OF PORTLAND CEMENT CONCRETE 1.0 GENERAL. 1.1 Scope
1.0 GENERAL 1.1 Scope 2.0 PRODUCTS 1.1.1 These specifications cover the requirements for the supply of Portland Cement Concrete to be used for all concrete work unless otherwise specified. The constituent
More informationSPECIAL APPLICATIONS CONCRETEPERVIOUS CONCRETE, PLASTIC CONCRETE AND CONTROLLED LOW STRENGTH MATERIAL
SPECIAL APPLICATIONS CONCRETEPERVIOUS CONCRETE, PLASTIC CONCRETE AND CONTROLLED LOW STRENGTH MATERIAL ABSTRACT V V Arora, P N Ojha, Suresh Kumar & Komalpreet Kaur National Council for Cement and Building
More informationDetermination of appropriate mix ratios for concrete grades using Nigerian Portlandlimestone grades 32.5 and 42.5
Leonardo Electronic Journal of Practices and Technologies ISSN 15831078 Issue 26, JanuaryJune 2015 p. 7988 Determination of appropriate mix ratios for concrete grades using Nigerian Portlandlimestone
More informationEnergy Absorbing Concrete for Impact Loading
Energy Absorbing Concrete for Impact Loading R. Sri Ravindrarajah * and M. C. Lyte ** *Senior Lecturer, **Former Student, Centre for Built Infrastructure Research University of Technology, Sydney, P O
More informationGreen Concrete by using Industrial Waste Material fly ash, quarry dust, marble powder
Green Concrete by using Industrial Waste Material fly ash, quarry dust, marble powder Santosh Kumbhar 1, Mahesh Patil 2, Dipak Patil 3 1,2,3 Students, Final year, Civil Engineering, SITCOE, Yadrav. Email:
More informationVOLUMETRIC MIXER STANDARDS OF THE VOLUMETRIC MIXER MANUFACTURERS BUREAU VMMB
VOLUMETRIC MIXER STANDARDS OF THE VOLUMETRIC MIXER MANUFACTURERS BUREAU VMMB 10001 First Edition February 28, 2001 Your Assurance of Quality! NEED HELP??? It is the policy of the Bureau to make its services
More informationKey Words Student Paper, Technology, Construction Management and Engineering Technology
Comparative Study of the Abrasion Resistance Radu Apostoaia, Purdue University Calumet Jose Pena, Purdue University Calumet Faculty Advisor: Jose A. Pena, Purdue University Calumet Student Paper Abstract
More informationEvaluation of the Physical and Chemical Properties of Fly Ash Products for Use in Portland Cement Concrete
2011 World of Coal Ash (WOCA) Conference May 912, 2011 in Denver, CO, USA http://www.flyash.info/ Evaluation of the Physical and Chemical Properties of Fly Ash Products for Use in Portland Cement Concrete
More informationMathematical Regression Model for the Prediction of Concrete Strength
Mathematical Regression Model for the Prediction of Concrete Strength M. F. M. Zain 1, Suhad M. Abd 1, K. Sopian 2, M. Jamil 1, CheAni A.I 1 1 Faculty of Engineering and Built Environment, 2 Solar Energy
More informationEffect of Vacuum Intrusion Compaction on the Mechanical Properties of Mortar
MAT EC Web of Conferences 17, 010 03 (2014) DOI: 10.1051/ matecconf/ 2014170100 3 C Owned by the authors, published by EDP Sciences, 2014 Effect of Vacuum Intrusion Compaction on the Mechanical Properties
More informationAbsorption and Specific Gravity. Specific Gravity
Absorption and Specific Gravity Specific Gravity Definition Ratio of the mass of a substance relative to the mass of an equal volume of water at a specified temperature. The density of water is 62.4 lb/ft3.
More informationEffects of Moisture Variation on Concrete Mixes and Methods to Control Final Mix Quality
10 th International Conference on Concrete Block Paving Shanghai, Peoples Republic of China, November 2426, 2012 Effects of Moisture Variation on Concrete Mixes and Methods to Control Final Mix Quality
More informationEvaluation of Initial Setting Time of Fresh Concrete
Evaluation of Initial Setting Time of Fresh Concrete R R C Piyasena, P A T S Premerathne, B T D Perera, S M A Nanayakkara Abstract According to ASTM 403C, initial setting time of concrete is measured based
More informationMechanical Properties of Rice Husk Ash Blended Cement Concretes made with OPC 53 Cement
Mechanical Properties of Rice Husk Ash Blended Cement Concretes made with OPC 53 Cement Srinivas K. 1, Kishore Kumar M 2 M.Tech Scholar, Department of Civil Engineering, Pydah College of Engineering, Visakhapatnam,
More informationUSE OF CONCRETE FAMILY CONCEPT FOR CONFORMITY CONTROL OF READY MIXED CONCRETE
USE OF CONCRETE FAMILY CONCEPT FOR CONFORMITY CONTROL OF READY MIXED CONCRETE Lu Jin Ping*, American Concrete Institute Singapore Chapter Soh Guan Hong, Admaterials Technologies Pte Ltd, Singapore Goh
More informationRECYCLED CRUSHED CONCRETE BASE COURSE
Section 02713 PART 1 G E N E R A L 1.01 SECTION INCLUDES A. Recycled crushed concrete base (RCCB) course. 1.02 MEASUREMENT AND PAYMENT A. Unit Prices. 1. Payment for RCCB is on per ton basis furnished
More informationUse of Recycled Concrete Aggregates in Structural Concrete in Mauritius
Journal of Emerging Trends in Engineering and Applied Sciences (JETEAS) 6(1): 7181 Scholarlink Research Institute Journals, 2014 (ISSN: 21417016) jeteas.scholarlinkresearch.com Journal of Emerging Trends
More informationSECTION 331 TYPE S ASPHALT CONCRETE
SECTION 331 TYPE S ASPHALT CONCRETE 3311 Description. Construct a Type SI, Type SII or Type SIII Asphalt Concrete as specified by the Contract. When offered as alternates, either Type may be constructed.
More informationSTUDY ON COMPRESSIVE STRENGTH OF CONCRETE BY USING TREATED DOMESTIC WASTE WATER AS MIXING AND CURING OF CONCRETE
STUDY ON COMPRESSIVE STRENGTH OF CONCRETE BY USING TREATED DOMESTIC WASTE WATER AS MIXING AND CURING OF CONCRETE Vinut Kulkarni 1, Suresh G Patil 2, Shivasharanappa 3 1 Mtech IV Sem (Environmental Engineering)
More informationcement Masonry Cement Engineered for quality and reliability, Lafarge cements for masonry deliver consistent performance. page 2 Lafarge Cement
cement Masonry Cement Engineered for quality and reliability, Lafarge cements for masonry deliver consistent performance. page 2 Lafarge Cement Lafarge in North America The Lafarge Group is the world leader
More informationManufacturing Quality Concrete Products
CEMEX USA  Technical Bulletin 8.0 Manufacturing Quality Concrete Products Establishing or Upgrading a Quality Program Overview The following guidelines were developed for MCP (manufactured concrete products)
More informationC. Section 014510 TESTING LABORATORY SERVICE.
SECTION 014500 QUALITY CONTROL PART 1 GENERAL 1.01 RELATED REQUIREMENTS A. Drawings and General Provisions of Contract, including General and Special Conditions and other Division 1 Specification Sections,
More informationStudies on Suitability of Fly Ash Based Cement Mortar Dry Mix with Quarry Dust as Fine Aggregate
International Journal of Scientific & Engineering Research, Volume, Issue 8, August ISSN 98 Studies on Suitability of Fly Ash Based Cement Mortar Dry Mix with Quarry Dust as Fine Aggregate Shefeena.N,
More informationThe AASHO Road Test site (which eventually became part of I80) at Ottawa, Illinois, was typical of northern climates (see Table 1).
Página 1 de 12 AASHO Road Test The AASHO Road Test, a $27 million (1960 dollars) investment and the largest road experiment of its time, was conceived and sponsored by the American Association of State
More informationSulfuric Acid Resistance of Concrete with Blast Furnace Slag Fine Aggregate
Nov. 2014, Volume 8, No. 11 (Serial No. 84), pp. 14031413 Journal of Civil Engineering and Architecture, ISSN 19347359, USA D DAVID PUBLISHING Sulfuric Acid Resistance of Concrete with Blast Furnace
More informationSECTION 18  CAST IN PLACE HIGH PERFORMANCE CONCRETE (HPC)
SECTION 18  CAST IN PLACE HIGH PERFORMANCE CONCRETE (HPC) 1.0 DESCRIPTION This section details the requirements for materials and methods in the proportioning, mixing, transporting, placing, finishing
More informationThe suitability of crushed over burnt bricks as coarse aggregates for concrete Apebo, N. S., Agunwamba, J. C., Ezeokonkwo, J. C.
The suitability of crushed over burnt bricks as coarse aggregates for concrete Apebo, N. S., Agunwamba, J. C., Ezeokonkwo, J. C. Abstract The research was conducted to study the suitability of crushed
More informationTesting and appraisal of Lucobit polymer effect as an additive on asphalt mixture performance
Abstract Testing and appraisal of polymer effect as an additive on asphalt mixture performance Hamid Sabbagh mollahosseini*,golazin Yadollahi**, Ershad Amoosoltani*** *, ***Executive of Engineering and
More informationSTATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENTAL SPECIFICATION 888 PORTLAND CEMENT CONCRETE PAVEMENT USING QC/QA.
STATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENTAL SPECIFICATION 888 PORTLAND CEMENT CONCRETE PAVEMENT USING QC/QA October 21, 2011 888.01 General 888.02 Materials 888.03 Concrete Proportioning 888.04
More informationDesigning effective sand and mortar mixes for Micro Concrete Roof Tiles (MCR)
Designing effective sand and mortar mixes for Micro Concrete Roof Tiles (MCR) Produced by Peter Dunckey Designing sand compositions for mcr tiles. To produce strong tiles, it is important to use clean
More informationA MIX DESIGN METHODOLOGY FOR CONCRETE BLOCK UNITS
A MIX DESIGN METHODOLOGY FOR CONCRETE BLOCK UNITS Frasson Jr., Artêmio 1 ; Casali, Juliana Machado 2 ; Oliveira, Alexandre Lima 3 ; Prudêncio Jr., Luiz Roberto 4 1 Master, Federal University of Santa Catarina,
More information